OPTICAL DENSITY AND PHOTONIC EFFICIENCY OF SILICA-SUPPORTED TiO2 PHOTOCATALYSTS
J. Marugán a, D. Hufschmidtb, G. Sagawe b, V. Selzer b, D. Bahnemann b *.
ESCET. Universidad Rey Juan Carlos. C/ Tulipán s/n, 28933 Móstoles, Madrid, Spain.
Universitaet Hannover. Institut fuer Technische Chemie (TCI). Callinstrasse 3, D-30167 Hannover, Germany.
Phone: +34 664 7466 ; Fax: +34 488 7068 ; E-Mail: email@example.com
Water Research, 40: 833-839 (2006).
Over the last years, many research groups have developed supported TiO2-based
materials in order to improve the engineering applications of photocatalytic technologies. However, not many attempts have been made to evaluate the optical behaviour of these materials. This work focuses on the study of the photonic efficiencies of silica-supported TiO2
photocatalysts following the photodegradation of dichloroacetic acid (DCA) as model compound. Catalysts with different types of silica support and titania loadings were tested and their activity was found to be in correlation with the results of the clusters size distribution of the TiO2 nanocrystals. The photonic efficiency of the supported photocatalysts depends
extremely on the optical density of the solid suspensions. Influence of the textural properties of the support and the titania loading on the optical density as well as on the photonic efficiency of the materials are discussed. The dependence of the absorption of radiation by the suspension on the catalyst concentration is also analyzed.
Keywords: Photocatalysis, photonic efficiency, optical density, supported TiO2,
TiO2 photocatalysis has been shown as an environmental-friendly technology for the
detoxification of industrial effluents. It has been shown that a large number of chemical pollutants are susceptible of being oxidized through heterogeneous photocatalytic processes (Ollis and Al-Ekabi, 1993; Blake, 1994a, 1994b, 1996, 1999, 2001; Hoffmann, 1995; Schiavello, 1997; Herrmann, 1999; Alfano et al., 2000). However, the commercial application of this method for the treatment of aqueous solutions is limited by both the recovery of the catalyst after the reaction and the economical feasibility of photocatalytic processes, conditioned by the efficiency in the use of the radiation. On this basis, many researchers have developed supported photocatalysts with suitable recovery and optimal light absorption properties (Pozzo et al., 1997; Byrne et al. 1998).
The results reported in the literature confirm a higher activity of powdered TiO2
compared with supported systems for most photocatalytic reactions. However, the need for down-streams processes to remove the catalyst is a strong motivation for the search of highly active supported photocatalysts. On the other hand, the use of a support can introduce diffusional restrictions to the mass transport of the pollutants (Chen et al. 2001) and hindrances to the light absorption by the semiconductor, thus reducing the overall photonic efficiency. For that reason, besides the conventional requirements of a support for heterogeneous catalysts, the materials used as supports for photocatalytic purposes must also fulfill stringent optical properties such as transparency to UV-A light, in order to achieve high photonic efficiencies and to minimize the energy consumption required for the illumination.
Despite the large number of supported TiO2 photocatalysts reported in the last years,
few attempts have been made to evaluate the optical behavior of these materials in terms of photonic efficiencies or quantum yields, optical parameters standardized by the IUPAC (Serpone and Salinaro, 1999; Salinaro et al. 1999). It is important to note that these parameters are absolutely required for the rigorous design and scaling-up of photocatalytic reactors in order to accomplish a commercial application of photocatalytic technologies (Curcó et al., 2002; Sagawe et al. 2003a, 2003b).
The goal of this work is to report the results obtained during the evaluation of the photonic efficiencies of several supported photocatalysts recently developed (van Grieken et al., 2002) and to compare them with those obtained employing commercially available
photocatalytic degradation of DCA has been studied extensively evincing that a single electron/hole pair suffices for its complete oxidation. The influence of different variables such as titania loading, type of silica support and catalyst concentration is discussed. One important conclusion of the work is that an unbiased comparison of the photoactivity of supported photocatalysts is not an easy task, because similar optical properties and semiconductor contents could not simultaneously achieved.
2. Materials and Methods
2.1. Catalyst synthesis and characterization
The synthesis procedure of the silica-supported TiO2 photocatalysts has been reported
elsewhere (van Grieken et al., 2002). Nanocrystalline clusters of TiO2 were obtained through
a sol-gel method, i.e., by the condensation of the required amount of titanium tetraisopropoxide inside the porous structure of the silica support. Different types of mesoporous silica materials have been used: an amorphous commercial SiO2 (Grace Sylopol
2104, GrSiO2) with a wide pore size distribution and the so-called SBA-15 silicas,
mesostructured materials with well defined pore sizes. The characterization of the samples shows differences in the textural properties and in the TiO2 crystal size depending on the TiO2
loading and the silica type (see table 1). More details about the synthesis, characterization and photoactivity of these materials are given elsewhere (van Grieken et al., 2002; Aguado et al., 2002; Lopez-Muñoz et al., 2005).
Table 1. Physical properties of the supported TiO2 photocatalysts.
BET surface (m2·g-1)
Pore volume (cm3·g-1)
BJH average pore size (nm) XRD average crystal size (nm)
GrSiO2 317 1.59 19.1 -
20%TiO2/GrSiO2 299 1.16 17.1 6.8
40%TiO2/GrSiO2 246 0.94 17.5 8.0
60%TiO2/GrSiO2 179 0.67 17.3 12.2
SBA-15 640 0.96 6.3 -
20%TiO2/SBA-15 532 0.33 6.0 6.2
40%TiO2/SBA-15 442 0.32 5.9 6.7
60%TiO2/SBA-15 349 0.18 5.8 6.8
SBA-15-TMB 601 1.62 12.4 -
2.2. Photocatalytic degradation test
Photodegradation experiments were carried out using a lamp field photoreactor with 64x110 cm2 of illuminated surface, covered with a light homogenizer of UV-A transparent glass and four perpendicular reflectors in order to obtain a frame of diffuse and homogeneous light (see figure 1). The emission spectra of the lamps (Phillips Cleo-R UV-A fluorescent lamps) are mainly centered in the 300-400 nm range. The photoreactor consisted of seven rectangular tubes (500x61x13 mm) made of polymethylmethacrylate (Plexiglas , Röhm GmbH, Darmstadt). Each tube was filled with 200 ml of the reaction suspension ten minutes after switching on the lamps, to ensure constant light emission. Both outer tubes were not used for reactions to avoid side-effects in the irradiation of the catalyst. Stirring and aeration was achieved by air bubbling through perforations in the bottom of each reactor tube. The incident photon flux measured by a Dr. Hönle UV-A sensitive photometer in the irradiated side of the photoreactor was 20 W m-2, equivalent to 6.0·10-5 Einstein m-2 s-1 as calculated for 365 nm wavelength radiation.
Figure 1. Schematic of the experimental setup: lateral view (left) and front view (right). (a) Fluorescent lamps (illuminating field), (b) homogenizer, (c) reflector, (d) supporting frame,
(e) photoreactor, (f) air sparging unit.
desired value (3, 7 or 10 depending on the desired reaction conditions) by addition of sodium hydroxide or nitric acid solutions, respectively. Samples were taken periodically to follow the degradation by chemical analysis after centrifugation. The geometry of the reactor assures the independence of the irradiation conditions during the successive withdrawal of solution, with a fixed relation between volume and irradiated surface area. The degree of the DCA photomineralization was determined by measuring the total organic carbon (TOC) concentration remaining in the clear solution by using a Shimadzu TOC-5000 analyzer. According to the accepted mechanism of DCA photocatalytic degradation (Ollis et al., 1984; Bahnemann et al., 2002), the TOC analysis provides the information of the remaining amount of reactant due to the absence of any stable intermediates during the total mineralization process.
The initial photonic efficiencies were calculated as = r0DCA (mol l-1 s-1) / I0 (Einstein
l-1 s-1), where r0DCA is the initial reaction rate as extrapolated from the DCA degradation
profile and I0 is the incident photon flow per volumetric unit (I0=4.64·10-6 Einstein l-1 s-1) determined by UV-A radiometric measurements. Consequently, the calculated values of are averaged on the wavelength spectrum of the lamp emission, centered in the range 300 – 400 nm.
3. Results and Discussion
3.1. Influence of the SiO2 support
Preliminary experiments were carried out at pH = 3 and 0.5 g l-1 of TiO2, in order to
compare the influence of the different silica supports at constant 20 wt% loading of titania. Figure 2 illustrates the TOC removal achieved with each supported photocatalyst as compared with the unsupported Degussa P25 commercial TiO2. The initial photonic efficiency
calculated for every catalyst is reported in Table 2. It can be seen that the activity shown by the Degussa P25 TiO2 powder is higher than the value observed with all of the supported
Figure 2. TOC removal during the photocatalytic degradation of 1 mM DCA (CCatal = 0.5 g
TiO2·l-1; I0 = 4.64·10-6 Einsteinl·l-1·s-1 ; pH = 3; T = 25ºC).
Table 2. Photonic efficiencies (molDCA Einstein-1) of the supported photocatalysts at different
3 7 12
Degussa P25 TiO2 0.080 0.059 0.017
20%TiO2/SBA-15 0.031 0.004 0.002
20%TiO2/SBA-15-TMB 0.026 0.012 0.004
20%TiO2/GrSiO2 0.021 0.008 0.003
Similar results have been previously obtained for the photoxidation of cyanides (van Grieken et al., 2002). The lower activity of the supported catalysts as compared with powdered TiO2 can either be explained in terms of a lower intrinsic activity of the TiO2
particles or by the existence of transport restrictions (of chemicals or photons) due to the support. Concerning the higher activity of the TiO2/SBA-15 photocatalyst, this fact has been
explained in terms of the well-defined TiO2 crystal size distribution obtained by using
SBA-15 silica as support (López-Muñoz et al., 2005) in comparison with the amorphous structure of the commercial silica or the too wide pore size of the SBA-15-TMB silica.
catalyst suspension placed inside the reactor. It is obvious that large differences of the UV-A transmittance were obtained depending on the catalyst. Whereas for Degussa P25 there is a complete absorption of the radiation under the employed reaction conditions, the absorption of the supported catalyst suspensions can be increased with higher catalyst concentration or by using a thicker reactor plate, thus probably improving their photoactivity.
Figure 3. Photonic efficiency for DCA photodegradation and UV-A transmittance of Degussa P25 and TiO2 supported on different silica materials (CCatal = 0.5 g TiO2·l-1; I0 = 4.64·10-6
Einsteinl·l-1·s-1 ; pH = 3; T = 25ºC).
Regarding the influence of the initial pH of the solution on the photonic efficiency, the study of the DCA photodegradation was carried out at initial pH values of 3, 7 and 10. It must be noticed that these are initial values and that the pH was not controlled during the reaction. Consequently, a decrease of the suspensions pH was noticed as the mineralization of DCA proceeds, especially when the initial pH was 7. The results shown in Table 2 confirm the dependence of the photonic efficiency reported previously (Lindner et al., 1997). According to these authors, the photocatalytic degradation of DCA is a photo-Kolbe process that takes place through the following reactions:
CHCl2 – COO – + h+ CHCl2 – COO·
CHCl2 – COO· ·CHCl2 + CO2
·Cl2HCO2 + e– CO2 + H+ + 2Cl–
Bahnemann et al. (1997) reported that the initial degradation step occurs with the valence band holes as the main oxidizing species. This process requires the DCA molecules to be adsorbed on the TiO2 surface. Taking into account that DCA is almost totally dissociated
in the tested pH range (pKa = 1.29), the interaction should be maximum in acid media, where
the TiO2 surface is positively charged.
From Table 2 it can be seen that the initial photonic efficiency of the catalyst Degussa P25 increases as the initial pH value decreases. In addition to that, the dependence of the activity on the pH of the solution observed for the supported photocatalysts shows the same trend as that obtained for the Degussa P25 TiO2 powder. Moreover, the initial reduction of the
DCA concentration in solution due to the adsorption equilibrium prior to the beginning of the reaction is found to be negligible in all cases, including experiments with P25. Consequently, despite the higher surface area of the supported photocatalysts, no evidence of a significant adsorption of DCA on the silica surface has been found. This is readily explained by the fact that the SiO2 surface is negatively charged over the entire pH-regime studied here thus
preventing a significant adsorption of the anionic DCA molecule. These results suggest that there is no change in the mechanism of the DCA photocatalytic degradation resulting from the presence of the silica support.
3.2. Influence of TiO2 loading
Figure 4 shows the results obtained for the initial photonic efficiencies measured for the DCA degradation and the change of UV-A transmittance with increasing TiO2 loadings on
SBA-15 and amorphous silica. It can be seen that a slightly higher activity for the DCA photoxidation is obtained with SBA-15 based materials as compared with amorphous silica based materials containing similar TiO2 loadings. Additionally, it is interesting to note that the
activity results of the amorphous silica based materials are almost independent on the TiO2
Figure 4. Influence of the titania loading on the initial photonic efficiency for DCA photodegradation and on the UV-A transmittance of the different catalyst suspensions (CCatal
= 0.5 g TiO2·l-1; I0 = 4.64·10-6 Einsteinl·l-1·s-1 ; pH = 3; T = 25ºC).
Concerning the UV-A transmittance results shown in Figure 4, since the TiO2
concentration and the optical path are the same for all the experiments, a higher UV-A transmittance is due to a lower optical density of the material. It should be noticed that the optical density of the catalysts decreases as the loading of TiO2 increases.
The analysis of the data does not show a correlation between the UV-A transmittance of every catalyst suspension and the photonic efficiency value. Whereas for the amorphous silica, the activity is, as expected, independent on the optical density, the rather weak maximum in the activity of the catalysts 40%TiO2/SBA-15 cannot be related with the
transmittance of the suspensions. It is important to notice that the TiO2 crystal size and the
intrinsic activity of the semiconductor in the SBA-15 supported materials is independent upon the TiO2 loading (van Grieken et al. 2002). Taking into account all these considerations, the
activity of the samples apparently does not only depend upon the intrinsic TiO2 activity and
In summary, the higher activity of the 40%TiO2/SBA-15 catalysts could probably be
due to a combination between a higher concentration of the active phase within the solid (increasing the absorption to scattering ratio of the radiation) and the lower diffusion rate in the highly-occupied channels of the 60%/SBA-15 photocatalyst.
3.3. Influence of catalyst concentration and optical density
In order to clarify the influence of the TiO2 concentration and the optical density on
the photonic efficiency for the DCA degradation, further studies have been performed varying the catalyst concentration. Figure 5 shows the results obtained with the different 20 wt% TiO2
supported catalyst and with Degussa P25 TiO2. Once again it is obvious that the photonic
efficiency for Degussa P25 TiO2 powder is higher than that obtained for the supported
catalysts in the tested range of TiO2 concentration (0.1 – 2.0 g l-1). However, it is worth
mentioning that whereas the catalyst Degussa P25 reaches at a concentration of 0.1 g l-1 of TiO2 80% of its maximum activity, the supported materials increase their activities up to four
times at higher concentrations of TiO2. Consequently, differences in activity between Degussa
P25 and the supported materials are reduced by increasing the TiO2 concentration.
Taking into account the values of UV-A transmittance for each catalyst suspension shown in Figure 5, the results could be explained in terms of the amount of radiation absorbed by the suspension of the catalysts. For Degussa P25, radiation extinction is complete at a TiO2
concentration of 0.5 g·l-1. This factor leads to a negligible increase in activity at higher TiO2
concentration values. On the other side, the optical density of the 20%TiO2/SBA-15-TMB and
20%TiO2/GrSiO2 suspensions is increased and thus the activity is improved as the TiO2
concentration increases. By contrast, the activity of the material 20%TiO2/SBA-15 is not
significantly increased at TiO2 concentrations higher than 0.5 g·l-1, because of the higher
Figure 5. Influence of the TiO2 concentration on the initial photonic efficiency for DCA
photodegradation and on the UV-A transmittance of the different catalyst suspensions (I0 = 4.64·10-6 Einsteinl·l-1·s-1 ; pH = 3; T = 25ºC).
Concerning the TiO2 loading, Figure 6 shows the dependence of both the photonic
efficiency and the UV-A transmittance on the catalyst concentration for catalysts supported on amorphous silica with different TiO2 loadings. In this case, differences in activity and
optical density are not pronounced. For catalyst concentrations above 0.5 g·l-1 of TiO2, a
slightly increase in the photonic efficiency is achieved by increasing the TiO2 loading of the
material. Based on the characterization data shown in table 1, it seems unlikely that differences in the intrinsic activity of the TiO2 crystals or in the diffusion rate for the mass
transport of the pollutant inside the porous structure of the support are responsible for the higher photonic efficiency of the materials as the TiO2 loading increases. Therefore the
optical properties of the materials are supposed to be the main factor affecting the activity of these supported catalysts. The UV-A transmittance data show that differences in the optical density of the materials are not sufficient to explain the higher photonic efficiency upon the increasing TiO2 loadings. Taking into account that a higher TiO2 loading requires less amount
behavior could be produced by an increase in the radiation absorption to scattering ratio. This conclusion is sustained by considering that only the semiconductor content produces the radiation absorption whereas the support particles act as scattering centers.
Figure 6. Influence of the TiO2 concentration and TiO2 loading over amorphous silica in the
initial photonic efficiency for DCA photodegradation and UV-A transmittance of the different catalyst suspensions (I0 = 4.64·10-6 Einsteinl·l-1·s-1 ; pH = 3; T = 25ºC).
Regarding the catalysts supported on SBA-15 silica, Figure 7 shows the influence of the catalyst concentration on the photonic efficiencies for DCA photodegradation for different TiO2 loadings. It is obvious that the activity of the materials is almost independent of the TiO2
loading at low catalysts concentrations. However, as the amount of catalyst increases, differences in activity become more significant and for 2.0 g·l-1 of TiO2 the photonic
efficiency of the catalyst 40%TiO2/SBA-15 is twice as high as the value observed with the
20%TiO2/SBA-15 material. Figure 7 also shows that the dependence of the UV-A
Figure 7. Influence of the TiO2 concentration and the TiO2 loading over SBA-15 silica on the
initial photonic efficiency for the DCA photodegradation and the UV-A transmittance of the different catalyst suspensions (I0 = 4.64·10-6 Einsteinl·l-1·s-1 ; pH = 3; T = 25ºC).
In summary, we can conclude that the higher optical density of the SBA-15 silica in comparison with the amorphous silica could not totally explain the higher activity of all the SBA-15 based photocatalysts as compared with the amorphous silica based materials. In addition, the narrower crystal size distribution achieved by using this mesostructured material seems to have an important effect.
Concerning the TiO2 loading, it can be concluded that, generally speaking, an increase
in the TiO2 content of the material leads to higher photonic efficiencies at constant TiO2
concentration due to the reduction in the scattering effects achieved by the use of less particles of the silica support. However, by using SBA-15 silica as support this beneficial effect at high TiO2 loading is counteracted by an increase in the diffusional problems, thus leading to the
fact that the catalyst 60%TiO2/SBA-15 is less photocatalytically active than the
It is important to point out that an unbiased comparison of the photoactivity of supported photocatalysts is not an easy task. Due to different scattering properties of the different catalysts preparation, the use of the same amount of light-absorbing semiconductor material cannot guarantee a correct evaluation of the photonic efficiencies. On the other hand, the use of different catalyst concentrations to ensure similar absorption of the incoming radiation within the reactor also fails to perform the comparison properly due to the different semiconductor content. These facts show the high importance of both the catalytic and the optical properties for the design of an optimal photoreactor.
Based upon our results, the photocatalyst 40%TiO2/SBA-15 shows the maximum
activity of all tested materials, independently on the catalyst concentration and therefore the transmittance of the suspension. This fact could imply the existence of an optimal choice of the support and the TiO2 loading in order to obtain an adequate TiO2 activity limiting the
detrimental effect of the radiation scattering caused by the silica particles and the diffusional restrictions inside the porous catalyst structure.
The authors thank “Consejería de Educación, Comunidad de Madrid” for the financial support of this research through the project “Contrato-Programa Grupos Estratégicos de Investigación” and “Ministerio de Ciencia y Tecnología” through the project PPQ2000-1287.
Aguado J., van Grieken R., López-Muñoz M.J. and Marugán J. (1996). Removal of cyanides in wastewater by supported TiO2-based photocatalysts. Catal. Today 75, 95-102.
Alfano O.M., Bahnemann D., Cassano A.E., Dillert R. and Goslich R. (2000). Photocatalysis in water environments using artificial and solar light. Catal. Today 58, 199-230.
Bahnemann D., Hilgendorff, M. and Memming, R. (1997). Charge carrier dynamics at TiO2 particles: Reactivity of free and trapped holes. J. Phys. Chem. B 101, 4265-4275.
Bahnemann D., Kholuiskaya S.N., Dillert R., Kulak A.I. and Kokorin A.I. (2002). Photodestruction of dichloroacetic acid catalyzed by nano-sized TiO2 particles. Appl. Catal. B
Blake D. (1994). Bibliography of work on the photocatalytic removal of hazardous compounds from water and air. (first update: October 1994; second update: October 1996; third update: January 1999; fourth update: October 2001), NREL, Golden, CO.
Byrne, J.A., Eggins, B.R., Brown, N.M.D., McKinney, B. and Rouse, M. (1998). Inmobilisation of TiO2 powder for the treatment of polluted water. Appl. Catal. B: Environ.
Chen, D., Li, F. and Ray, A.K. (2001). External and internal mass transfer effect on photocatalytic degradation. Catal. Today 66, 475-485.
Curcó D., Giménez J. Addardak A., Cervera-March S. and Esplugas S. (2002). Effects of radiation absorption and catalyst concentration on the photocatalytic degradation of pollutants. Catal. Today 76, 177-188.
Herrmann J.M. (1999). Heterogeneous photocatalysis: fundamentals and applications to the removal of various types of aqueous pollutants. Catal. Today 53, 115-129.
Hoffmann M.R., Martin S.T., Choi, W. and Bahnemann D.W. (1995). Environmental applications of semiconductor photocatalysis. Chem. Rev. 95, 69-96.
Lindner M., Bahnemann D.W., Hirthe B. and Griebler W.-D. (1997). Solar water detoxification: Novel TiO2 powders as highly active photocatalysts. J. Solar Energy Eng. 119,
Lopez-Muñoz, M.J, van Grieken, R., Aguado, J. and Marugán, J. (2005). Role of the support on the activity of silica-supported TiO2 photocatalysts: structure of the TiO2/SBA-15
photocatalysts. Catal. Today 101, 307-314.
Ollis D.F., Hsiao C.Y., Budiman L. and Lee C.L. (1984). Heterogeneous photoassisted catalysis: conversions of perchloroethylene, dichloroethane, chloroacetic acids and chlorobenzenes. J. Catal. 88, 89-96.
Ollis D.F. and Al-Ekabi. (Eds.) (1993). Photocatalytic Purification and Treatment of Water and Air. Elsevier, Amsterdam.
Pozzo R.L., Baltanás M.A. and Cassano, A.E. (1997). Supported titanium oxide as photocatalyst in water decontamination: State of the art. Catal. Today 39, 219-231.
Sagawe G., Brandi, R.J., Bahnemann, D. and Cassano, A.E. (2003a). Photocatalytic reactors for treating water pollution with solar illumination. I: A simplified analysis for batch reactors. Chem. Eng. Sci. 58, 2587-2599.
Salinaro, A., Emeline, A.V., Zhao, J., Hidaka, H., Ryabchuk, V.K. and Serpone, N. (1999). Terminology, relative photonic efficiencies and quantum yields in heterogeneous photocatalysis. Part II: Experimental determination of quantum yields. Pure & Appl. Chem. 71, 321-335.
Schiavello, M. (Ed.) (1997). Heterogeneous Photocatalysis. Wiley, New York.
Serpone, N. and Salinaro, A. (1999). Terminology, relative photonic efficiencies and quantum yields in heterogeneous photocatalysis. Part I: Suggested protocol. Pure & Appl. Chem. 71, 303-320.
van Grieken R., Aguado J., López-Muñoz M.J. and Marugán J. (2002). Synthesis of size-controlled silica-supported TiO2 photocatalysts. J. Photochem. Photobiol. A 148,